towards a highly accessible and hydrostable MOF-phase within hybrid polyHIPEs through in situ metal-oxide recrystallization †

HKUST-1(Cu) and MOF-5(Zn)@polyHIPE hybrid materials were prepared using a metal salt-free technique, wherein metal–organic frameworks were in situ generated from the CuOand ZnO-nanoparticles through secondary recrystallization. The solid-to-MOF transformation has proven to be a feasible and effective technique for preparingMOF@polyHIPE hybridmaterials with a highMOF content of more than 75 wt%. The MOF phase within the hybrid polyHIPEs as disclosed herein exhibits superior micropore accessibility, structure hydrostability and durable CO2 adsorption capacity under humid conditions, not achievable with any of the previously reported methods.

Porous metal-organic frameworks (MOFs), crystalline solids with a well-dened porous structure, are a rapidly emerging class of multifunctional materials, which can be applied in various elds of physical and chemical processing. 1 Utilization of potentially useful MOFs is oen hindered due to the low hydrostability or the challenges of shaping. 2 To widen the practical utility of MOFs and enhance their durability, synthetic strategies that will deliver MOFs in a new, application-specic congurations are vital.Several bottom-up (using pre-formed templates) 3 and top-down (using pre-synthesised MOFs) 4 synthetic strategies of shaping have been already applied.A signicant amount of effort was made in depositing MOFs nanocrystals onto porous substrates like ceramic, 5 silica, 6 alumina 7 or within the mixed-matrix membrane (MMM) systems. 8Embedding MOFs into the organic (polymeric) matrices is an appealing combination while hybrids maintain the shape and exibility of the polymeric supports and exhibit the microporosity and high surface area of MOFs.Particularly interesting are microcellular polymeric foams as matrices, since their macropores serve as "highways" providing an unobstructed ow for hosting molecules that are aiming to access active-sites within the MOF's microporosity.Pore geometry, sizes and surface functionalities in porous polymeric matrices can easily be adjusted through one of the various methodologies. 9Among the methodologies available for preparing porous polymers, high internal phase emulsion (HIPE) templating and polyHIPEs thereof are especially intriguing. 10The major advantage of polyHIPEs is very high porosity (between 74 and 95 vol%) and unique void and window structures that are highly 3D-interconnected with voids typically between 5 and 20 mm in diameter.A number of hybrids based on various MOFs and polyHIPEs have been developed through different synthetic routes: conventional solvothermal synthesis of the MOFs within the pre-formed polyHIPEs, 11,12 incorporation of pre-formed MOFs into the HIPEs following polymerization, 13 and simultaneous formation of MOFs and polyHIPEs. 14However, the hybrids designed by these three approaches are all facing the same problems associated with the MOF phase (i) chemical and hydrolytic instability in monomeric solutions, (ii) low loadings and (iii) micropore clogging.Recently, an efficient synthetic strategy, the so-called seeded growth, has been introduced for the MOF synthesis, where nano-or microparticles were used as seeds that nucleate the MOFs. 15Seed deposition offers the ability to use particles (e.g.metal-oxides) to locate the MOF nucleation and growth in preferential areas.
Herein, we extend the concept of seeded growth strategy to the MOFs@polyHIPE hybrids for the rst time, by using preformed metal-oxide@polyHIPE nanocomposites.Key for this endeavour is the use of metal-oxide nanoparticles (MO x -NPs) embedded within the polymer walls as seeds and as metal ion reservoirs for MOF growth in the presence of appropriate organic ligands (i.e.BTC ¼ 1,3,5-benzenetricarboxylic acid or BDC ¼ 1,4-benzenedicarboxylic acid).The synthetic approach as disclosed herein has several advantages over the existing ones regarding MOFs: (i) the micropore clogging by the emulsion components is negligible, yielding high sorption accessibility aer polymerization; (ii) MOF stability in HIPEs is no longer an issue, since the direct contact with the monomeric solution is avoided.This allows very sensitive MOF systems to be incorporated into polyHIPE; (iii) MOF loading is conditioned by the content of MO x -NPs within the hybrid that can be very high (up to 40 wt% according to the monomers).
First, microcellular nanocomposite foams (mCNF) based on ZnO and CuO NPs were prepared according to the protocols recently published. 16A mixture of dicyclopentadiene (DCPD; 20 vol%) as a monomer, oleic acid coated NPs (30 wt% of NPs according to the monomer, Table S1 †), and surfactant Pluronic L-121 (7 vol% according to monomer) as a stabilizer were used as the organic (continuous) phase, while the internal (droplet) phase was deionized water (80 vol%).This formulation was subsequently polymerized upon the addition of the ringopening metathesis polymerization (ROMP) initiator (M2, see Scheme 1).The porous structures of the puried and dried mCNF were characterized using scanning electron microscopy (SEM).The mCNF exhibited the highly interconnected, opencell, porous structures typical of polyHIPEs, as seen in Fig. 1C  and D. The void and the interconnecting window diameters are around 7 and 2 mm, respectively.Aerwards, Cu-and Zn-based MOFs were successfully recrystallized under the solvothermal conditions from the corresponding mCNF into the HKUST-1(Cu) @polyHIPE and MOF-5(Zn)@polyHIPE hybrids.Scanning electron microscopy (SEM) revealed the fully preserved polyHIPE morphology with octahedral (HKUST-1) or cubic (MOF-5) shaped crystallites, embedded within the void walls (Fig. 1A and B).PolyHIPE's void and window sizes remain in the same range as they were before the recrystallization.
MO x -NPs are completely recrystallized into the MOF phase as evidenced by XRD (Fig. 2 and S1 †), which reveal no visible diffraction peaks belonging to the corresponding MO x in any case.However, broadening of the XRD peaks and increased background of the composite patterns can result in the overestimation of the MOF recrystallization rate due to the potential overlapping of the peaks corresponding to the metal oxides.Therefore, TGA was performed to determine the MOF contents within the hybrids as well as to cross-check the recrystallization efficiency (Fig. S2 and S3 †).Taking into account the MOF-5 formula, i.e.Zn 4 O(BDC) 3 , the solvent content, and the total weight loss of ZnO mCNF (78.1 wt%), the theoretical amount of MOF-5 aer complete recrystallization should be 55.1 wt% (Fig. S2 and S3 †).The TGA of the MOF-5@polyHIPE hybrid material shows a weight loss of 24% due to the solvent removal and 57.8 wt% due to the decomposition of organic compounds.The calculated amount of the MOF-5 in the hybrid material perfectly matches the theoretical value of 55.1 wt%.The measured amount of HKUST-1 within the hybrid material was found to be 75.4wt% and thus almost attains the theoretical value extracted from the thermogram of the CuO mCNF hybrid material (76.5 wt%).Higher contribution of HKUST-1 within the polyHIPE matrix can be explained by higher CuO loading within the polyHIPE (28 wt% for CuO vs. 22 wt% for ZnO).TGA conrmed almost complete transformation of the MO x -NPs into the MOF phase in both cases as it was already suggested by XRD measurements.Integration of MOFs within the polyHIPE matrix provides the opportunity to retain MOF's high porosity and accessibility for hosting molecules which is very important in applications such as catalysis or gas storage and separation. 11owever, avoiding micropore blocking through the preparation of MOF@polyHIPE hybrid materials remains a big challenge.Secondary recrystallization as disclosed herein seems to be a promising solution.Pure HKUST-1 and MOF-5 powders show typical type I isotherm as determined by the BET method with the specic surface areas (S BET ) of 1211 and 2501 m 2 g À1 for HKUST-1 and MOF-5, respectively.On the other hand, the pure mCNFs have negligible surface areas with no accessible microporosity.Aer recrystallization of the mCNFs the S BET of newly obtained hybrid materials increases signicantly.In both cases, S BET shows about half of the values as were measured for the parent MOF materials, i.e. 794 and 1298 m 2 g À1 for the HKUST-1@polyHIPE and MOF-5@polyHIPE, respectively.In both cases, the isotherms show a signicant increase of the N 2 uptake in the p/p o region up to 0.1, which can be assigned to the presence of the micropores.The MOF-5@polyHIPE hybrid material further exhibits a small hysteresis loop in the p/p o region between 0.85 and 1.0 most possibly due to the new mesopores created in the intercrystalline space of the MOF-5 or the interparticle space between MOF-5 crystals and the polyHIPE framework (Fig. 3).The drop of the surface area of hybrid materials goes mainly on the expense of the polyHIPE matrix presence, which does not contain any measurable microporosity.Moreover, secondary recrystallization is a post-polymerization process in which no emulsion components can clog the micropores.Therefore, it is sensible to suspect that the polymer matrix itself partially blocks the entry into the micropores.In order to estimate the quantity of the potentially blocked micropores the accessibility of MOF sorption sites, which is dened as a ratio between measured and expected BET surface areas, was calculated.The expected surface area was calculated taking into account the S BET of the parent MOFs and their weight contribution within the hybrids (see ESI †).The micropores' accessibility was found to the large extent unobstructed.HKUST-1@polyHIPE and MOF-5@polyHIPE hybrids exhibited 86% and 93% of the accessible micropores, respectively, which are among the highest values published for the MOF@polyHIPE hybrid materials (Table S2 †).Slightly lower accessibility in the case of HKUST-1@polyHIPE can be related to the fact that the HKUST-1 crystals are more embedded within the polymer matrix as can be seen from the SEM micrographs (Fig. 1A and B).
MOF-5 and HKUST-1 crystals are known to exhibit high structure sensitivity towards moisture, which in large extent limits their applicability in various physical or chemical processes.Hydrostability was investigated for the synthesized hybrids in order to evaluate their functionalities under humid conditions.The hybrid materials and the parent MOFs were exposed to 98% of relative humidity for 3 days at room temperature.Both parent MOFs underwent the hydrolysis process already aer 24 h, which is manifested in the case of HKUST-1 by signicant reduction of crystallinity and appearance of additional nonporous phase, whereas the structure of MOF-5 is completely recrystallized as can be seen from the  XRDs (Fig. S1 †). 17 On the other hand, the HKUST-1 and MOF-5 phases within the hybrid materials remained unchanged (Fig. S1 †).A slight decrease of the reection intensities and broadening of the peaks indicate partial amorphization of the MOF phase, however, the nonporous hydrous phase which commonly forms from the bulk MOF-5 did not occur.The N 2 isotherms are consistent with the XRD results.The exposure of the HKUST-1@polyHIPE hybrid material in a humid environment did not have any signicant negative effect on the porosity as indicated by only a slight decrease in the S BET of the humidity treated sample (from 794 to 777 m 2 g À1 ).The deterioration of the porosity is somewhat more pronounced in the case of MOF-5@polyHIPE aer humidity tests, wherein S BET decreases for about 30% (from 1298 to 910 m 2 g À1 ) (Fig. S4 †).The reason for such a profound improvement of the MOF hydrostability is due to the inherently hydrophobic nature of the poly(DCPD) poly-HIPE that repels the water vapour and protects the MOFs.
HKUST-1@polyHIPE and MOF-5@polyHIPE hybrid materials were further tested for the CO 2 uptake under humid conditions.CO 2 capture under the realistic conditions, e.g.CO 2 removal from ue gases, includes also the presence of other components (most notably 5-7% water vapour). 18While the presence of water vapour signicantly reduces the CO 2 adsorption capacity of the promising porous materials, most of the CO 2 adsorption tests are done under dry conditions. 19In our case, CO 2 cycling experiments were performed under sequential CO 2 adsorption at 1 bar and 25 C followed by exposure to 50% humidity.Both hybrid materials, i.e.HKUST-1@polyHIPE and MOF-5@polyHIPE (Fig. 4B and D), showed high durability.Aer 20 cycles, the CO 2 sorption capacity of the HKUST-1@polyHIPE remained constant at around 108 mg g À1 .In the case of MOF-5@polyHIPE the capacity decreases for about 35% (from 38 to 25 mg g À1 ), which is consistent with the loss of porosity as revealed by N 2 sorption analysis.On the contrary, the parent HKUST-1 was continuously losing the ability to adsorb CO 2 and aer 20 cycles exhibited only approximately 40% of the initial capacity.In the case of parent MOF-5, the decrease was even more pronounced and aer 5 cycles the adsorption capacity became negligible, indicating its complete transformation into nonporous hydrous Zn-terephthalate.

Conclusions
A new synthetic route to prepare MOF@polyHIPE hybrid materials via secondary recrystallization of the pre-synthesized metal-oxide@polyHIPE nanocomposites is disclosed.This synthetic approach is a step forward in the MOF@polymer heterostructure design.It overcomes the issues of limited loadings, chemical instability and micropore clogging associated with the MOF phase once incorporated into the polymer framework.By avoiding a direct contact between the MOFs and the monomeric solution, we enable the incorporation of various sensible (unstable) MOFs into a polyHIPE structure.Referring to the advantages of the secondary recrystallization approach, the HKUST-1@polyHIPE and MOF-5@polyHIPE hybrid materials were synthesized and exhibit a high MOF phase loading with pronounced micropore accessibility.Both hybrid materials further show improved structure resistivity upon water vapour exposure, offering the functionality of the water-sensitive MOF hybrid materials under humid conditions.The structure-function relationship of the newly obtained hybrid material under humid conditions was further tested for CO 2 uptake/exposure to 50% humidity cycling.Aer 20 cycles, the CO 2 sorption capacity of the hybrid MOF@polyHIPE materials does not change signicantly, showing high synergism of both components constituting the hybrid materials.

Scheme 1
Scheme 1 Schematic representation of the MOF nanocrystals grown through the secondary recrystallization of the MO x -NPs within the polyHIPEs.